Template Synthesis of Three-Dimensional Cubic Ordered Mesoporous Carbon With Tunable Pore Sizes
© to the authors 2009
Received: 30 July 2009
Accepted: 24 September 2009
Published: 14 October 2009
Three-dimensional cubic ordered mesoporous carbons with tunable pore sizes have been synthesized by using cubic Ia3d mesoporous KIT-6 silica as the hard template and boric acid as the pore expanding agent. The prepared ordered mesoporous carbons were characterized by powder X-ray diffraction, scanning electron microscopy, transmission electron microscopy, and nitrogen adsorption–desorption analysis. The results show that the pore sizes of the prepared ordered mesoporous carbons with three-dimensional cubic structure can be regulated in the range of 3.9–9.4 nm. A simplified model was proposed to analyze the tailored pore sizes of the prepared ordered mesoporous carbons on the basis of the structural parameters of the silica template.
In recent years, ordered mesoporous carbons (OMCs) with uniform pore sizes, high surface areas, and large pore volumes have been of wide interest for applications in many fields, such as catalyst supports, adsorbents, fuel cells, and electrodes for supercapacitors [1–3]. The hard template method has been successfully developed in the synthesis of OMCs. Since the emergence of numerous mesoporous silica materials, OMCs with various pore structures and narrow pore size distributions have been achieved by replicating the structures of mesoporous silica materials. The first OMC, CMK-1, was synthesized by Ryoo et al.  using MCM-48 silica (Ia3d) as a hard template. After that, ordered mesoporous silica materials with diverse symmetries, such as SBA-15 (p6mm) [5, 6], SBA-16 (Im3m) , KIT-6 (Ia3d) [7, 8], and FDU-12 (Fm3m) , were also employed to prepare OMCs.
The hard template synthesis procedure of OMCs involves impregnation of the silica template, carbonization of the carbon precursor, and removal of the silica template . The structure of the OMC, such as the pore shape and the pore size, was determined by the silica template. It is believed that OMCs with tunable pore size distributions would be beneficial for various applications. Ryoo et al. reported the synthesis of mesoporous silicas with controllable pore wall thicknesses of 1.4–2.2 nm, which were further used as templates to synthesize OMCs with tailored pore diameters of 2.2–3.3 nm . Alvarez et al.  modulated the pore sizes of mesoporous carbons within the range of 2–10 nm by changing the synthesis temperature of the silica template. However, the synthesis procedures of silica templates with different properties were tedious and difficult to precisely control.
Recently, Lee et al.  reported the synthesis of two-dimensional (2-D) hexagonal OMCs with controllable pore sizes in the range of 3–10 nm using MSU-H silica as the hard template and boric acid as the pore expanding agent, which was considered to be a facile method for the pore size control of OMCs. The pore expansion was realized by the spontaneous phase separation of the boron species from the boron and carbon precursors to the silica surface. Besides, the pore size was determined by the amount of the boric acid added to the carbon precursor. Herein, on the basis of this method, we report the synthesis of three-dimensional (3-D) cubic OMCs with tunable pore size distributions using KIT-6 silica as the template and boric acid as the pore expanding agent. Compared with MSU-H silica, KIT-6 silica exhibits 3-D cubic structure with Ia3d symmetry, which consists of the interpenetrating bicontinuous channel networks. We demonstrated that the aforementioned synthesis pathway could be generalized to prepare OMCs with various structures and symmetries using different mesoporous silicas as templates. Moreover, we quantitatively analyzed the pore expansion mechanism using a simplified model on the basis of structural parameters of the silica template.
The poly(alkylene oxide)-based triblock copolymer Pluronic P123 (EO20PO70EO20, MW = 5,800) and tetraethyl orthosilicate (TEOS, 98 wt%) were purchased from Aldrich Chemical Inc. Other chemicals were purchased from Shanghai Chemical Corp. All chemicals were used as received without further purification.
Synthesis of KIT-6 Silica
The synthesis of mesoporous KIT-6 silica with cubic Ia3d symmetry was performed according to the literature procedure reported elsewhere . Typically, 5 g of Pluronic P123 was dissolved in 180 g of distilled water and 9.9 g of HCl solution (35 wt%) under vigorous stirring at 35°C. After complete dissolution, 5 g of n-butanol (99.4 wt%) was added. Following further stirring for 1 h, 10.75 g of TEOS was added immediately. Subsequently the mixture was left stirring at 35°C for 24 h and transferred into an autoclave, which was sealed and maintained at 100°C for another 24 h under static conditions. The resulting solid product was filtered and dried at 100°C overnight. After a brief ethanol/HCl washing, the final sample was dried at 70°C and calcined at 550°C for 6 h in air.
Synthesis of Ordered Mesoporous Carbons
Ordered mesoporous carbon materials were synthesized using the recipe described previously [4, 12]. KIT-6 and sucrose were used as the template and the carbon precursor, respectively. Various amount of boric acid were added to the carbon precursor while keeping the sucrose concentration constant. The carbon replicas were designated as OMC-x, where x stands for the molar ratio of boric acid to sucrose. In a typical synthesis of OMC-1, 0.113 g of boric acid (99.5 wt%), 0.625 g of sucrose (95 wt%), and 0.071 g of sulfuric acid (98 wt%) were dissolved in 2.5 g of distilled water. After 0.5 g of KIT-6 silica was added, the mixture was heated at 100°C for 6 h, and subsequently at 160°C for another 6 h. The resulted composite was impregnated again with an aqueous solution consisting of 0.075 g of boric acid, 0.413 g of sucrose, 0.047 g of sulfuric acid, and 2.5 g of distilled water. After the heat treatment at 100°C and 160°C once again as before, the composite was carbonized at 900°C for 3 h under N2 flow. Finally, the OMC-1 material was obtained by the removal of the silica template using 5 wt% HF solution at room temperature.
Low-angle X-ray diffraction (XRD) was carried out on a Bruker D8 advance X-ray diffractometer using Cu Kα radiation. Scanning electron microscopy (SEM) images were obtained with a Hitachi S-4800 scanning electron microscope operating at 10 kV. Transmission electron microscopy (TEM) images were taken on a JEOL JEM-2100 microscope operated at 200 kV. Nitrogen adsorption–desorption isotherms were measured on a Micromeritics ASAP 2010 volumetric adsorption analyzer at 77 K.
Results and Discussion
Structural properties of KIT-6 silica and the OMCs
According to the Eq. 1, the pore diameters of OMC-1, OMC-4, OMC-8, and OMC-12 are estimated to be 4.85–5.2, 5.65–5.96, 6.3–6.57, 6.71–6.96 nm, respectively. The estimated values are mainly coincident with the data shown in Table 1 except for OMC-12, which exhibits a greatly broader pore size distribution due to the structural deterioration.
On the basis of the unit cell parameter and the pore diameter of KIT-6 silica, we estimated the pore diameter of the prepared OMC. OMCs with more precisely controlled pore sizes can be synthesized according to the estimated values calculated from the Eq. 1with proper molar ratio of boric acid to sucrose. It should be noted that the aforementioned derivation is simplified. The practical volume changes during the carbonization and the spontaneous phase separation of the boron species were neglected. Moreover, the pore size analysis performed using the BJH method is applicable for cylindrical mesopores [16, 17], whereas the inverse carbon replica of KIT-6 exhibits rod-type structure . It results in the overestimation of the pore widths of the prepared OMCs, which was also ignored in the derivation.
In summary, we synthesized 3-D cubic OMCs with tunable pore sizes in the range of 3.9–9.4 nm by using KIT-6 silica as the hard template and boric acid as the pore expanding agent. The pore expansion method reported by Lee et al. was demonstrated to be effective on the preparation of OMCs with different pore symmetries and tunable pore sizes. According to a simplified model, we deduced the carbon pore size equation that is expected to direct the synthesis of OMCs with tunable pore sizes on the basis of this synthesis pathway. The present work is expected to be helpful for the synthesis of OMCs with other pore structures by using other kinds of silica templates. Further, the practical application of the prepared 3-D cubic OMCs in energy storage is under investigation and will be reported in the future.
This work was supported by National Science Foundation of Jiangsu Province (BK2006195), Doctor Innovation Funds of Jiangsu Province (BCXJ06-13), and National Natural Science Foundation of China (50502020, 50701024).
- Liang CD, Li ZJ, Dai S: Angew. Chem. Int. Ed.. 2008, 47: 3696. COI number [1:CAS:528:DC%2BD1cXmsVKiurY%3D] COI number [1:CAS:528:DC%2BD1cXmsVKiurY%3D] 10.1002/anie.200702046View ArticleGoogle Scholar
- Lee J, Kim J, Hyeon T: Adv. Mater.. 2006, 18: 2073. COI number [1:CAS:528:DC%2BD28Xptlygs7k%3D] COI number [1:CAS:528:DC%2BD28Xptlygs7k%3D] 10.1002/adma.200501576View ArticleGoogle Scholar
- Stein A, Wang ZY, Fierke MA: Adv. Mater.. 2009, 21: 265. COI number [1:CAS:528:DC%2BD1MXhsleqtbg%3D] COI number [1:CAS:528:DC%2BD1MXhsleqtbg%3D] 10.1002/adma.200801492View ArticleGoogle Scholar
- Ryoo R, Joo SH, Jun S: J. Phys. Chem. B. 1999, 103: 7743. COI number [1:CAS:528:DyaK1MXltlyqu7o%3D] COI number [1:CAS:528:DyaK1MXltlyqu7o%3D] 10.1021/jp991673aView ArticleGoogle Scholar
- Zhao DY, Feng JL, Huo QS, Melosh N, Fredrickson GH, Chmelka BF, Stucky GD: Science. 1998, 279: 548. COI number [1:CAS:528:DyaK1cXotVOitQ%3D%3D]; Bibcode number [1998Sci...279..548Z] COI number [1:CAS:528:DyaK1cXotVOitQ%3D%3D]; Bibcode number [1998Sci...279..548Z] 10.1126/science.279.5350.548View ArticleGoogle Scholar
- Zhao DY, Huo QS, Feng JL, Chmelka BF, Stucky GD: J. Am. Chem. Soc.. 1998, 120: 6024. COI number [1:CAS:528:DyaK1cXjslKnsbY%3D] COI number [1:CAS:528:DyaK1cXjslKnsbY%3D] 10.1021/ja974025iView ArticleGoogle Scholar
- Kleitz F, Choi SH, Ryoo R: Chem. Commun.. 2003, 17: 2136. 10.1039/b306504aView ArticleGoogle Scholar
- Kim TW, Kleitz F, Paul B, Ryoo R: J. Am. Chem. Soc.. 2005, 127: 7601. COI number [1:CAS:528:DC%2BD2MXjsFyisrs%3D] COI number [1:CAS:528:DC%2BD2MXjsFyisrs%3D] 10.1021/ja042601mView ArticleGoogle Scholar
- Fan J, Yu CZ, Gao T, Lei J, Tian BZ, Wang LM, Luo Q, Tu B, Zhou WZ, Zhao DY: Angew. Chem. Int. Ed.. 2003, 42: 3146. COI number [1:CAS:528:DC%2BD3sXlvF2hsb8%3D] COI number [1:CAS:528:DC%2BD3sXlvF2hsb8%3D] 10.1002/anie.200351027View ArticleGoogle Scholar
- Lee JS, Joo SH, Ryoo R: J. Am. Chem. Soc.. 2002, 124: 1156. COI number [1:CAS:528:DC%2BD38XntlOlsQ%3D%3D] COI number [1:CAS:528:DC%2BD38XntlOlsQ%3D%3D] 10.1021/ja012333hView ArticleGoogle Scholar
- Alvarez S, Fuertes AB: Carbon. 2004, 42: 433. COI number [1:CAS:528:DC%2BD2cXislSqsA%3D%3D] COI number [1:CAS:528:DC%2BD2cXislSqsA%3D%3D] 10.1016/j.carbon.2003.10.035View ArticleGoogle Scholar
- Lee HI, Kim JH, You DJ, Lee JE, Kim JM, Ahn WS, Pak C, Joo SH, Chang H, Seung DY: Adv. Mater.. 2008, 20: 757. COI number [1:CAS:528:DC%2BD1cXlt1WmsrY%3D] COI number [1:CAS:528:DC%2BD1cXlt1WmsrY%3D] 10.1002/adma.200702209View ArticleGoogle Scholar
- Gierszal KP, Kim TW, Ryoo R, Jaroniec M: J. Phys. Chem. B. 2005, 109: 23263. COI number [1:CAS:528:DC%2BD2MXht1ajsrjF] COI number [1:CAS:528:DC%2BD2MXht1ajsrjF] 10.1021/jp054562mView ArticleGoogle Scholar
- Gierszal KP, Jaroniec M, Kim TW, Kim J, Ryoo R: New J. Chem.. 2008, 32: 981. COI number [1:CAS:528:DC%2BD1cXmvFGltLk%3D] COI number [1:CAS:528:DC%2BD1cXmvFGltLk%3D] 10.1039/b716735kView ArticleGoogle Scholar
- Kim TW, Solovyov LA: J. Mater. Chem.. 2006, 16: 1445. COI number [1:CAS:528:DC%2BD28Xkt1Gmsbo%3D] COI number [1:CAS:528:DC%2BD28Xkt1Gmsbo%3D] 10.1039/b516945cView ArticleGoogle Scholar
- Kruk M, Jaroniec M, Sayari A: Langmuir. 1997, 13: 6267. COI number [1:CAS:528:DyaK2sXmvVakur0%3D] COI number [1:CAS:528:DyaK2sXmvVakur0%3D] 10.1021/la970776mView ArticleGoogle Scholar
- Kim TW, Ryoo R, Gierszal KP, Jaroniec M, Solovyov LA, Sakamoto Y, Terasaki OJ: J. Mater. Chem.. 2005, 15: 1560. COI number [1:CAS:528:DC%2BD2MXjtV2gtrs%3D] COI number [1:CAS:528:DC%2BD2MXjtV2gtrs%3D] 10.1039/b417804aView ArticleGoogle Scholar